Synthesis and Application of Nanosize Semiconductors for Photoxidation of Toxic Organic Chemicals. J.P. Wilcoxon, Nanostructures and Advanced Materials Chemistry Sandia National Laboratories Albuquerque, N.M ., 87185-1421 [email protected]
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Nanostructures and Advanced Materials Chemistry
Sandia National Laboratories
Albuquerque, N.M., 87185-1421
Colloborators: T.R. Thurston, P. Provencio, G.A. Samara
Organic Pool in Soil
Step 1: Excavation, Soil Washing
Conventional Treatment Options:
1)Filtration and/or Adsorption of toxic chemicals in aqueous supernatant from Step 1
2)Chemical Oxidation or Total Mineralization of the the Organics
3)Deep UV Photooxidation of the Organics
4)Photocatalytic oxidation of the Organics (e.g. colloidal titania slurries)
- - - -
CO2 + HCl
+ + + +
1) Efficient conversion of sunlight to electron-hole pairs.
2) Surface trapping of electrons and holes before recombination.
3) Catalyst photostability.
4) Inexpensive, chemically-stable, environmentally benign materials.
weak van-der-Waals forces
Ionic II-VI Materials
Carrier Excitation Weakens
Covalent Semi-conductors (Stable)
Chemical Bonds (Unstable)
Mo, 4 dz
Synthesis in Inverse Micelle System
Mo4+ + 2S2- = MoS2
Mo Source: MoCl4, S Source: H2S, Oil: Octane
Typical Surfactant: Tri-ocytlmethylammonium Chloride (TOAC)
With hydrophilic cationic Surfactant
With Hydrophobic TOAC Surfactant
1) Liquid Chromatography shows the MoS2 clusters have a net charge.
2) Samples diluted into water are dialized to remove unwanted ions like SO4-2
3) Analysis by XRF gives the final [Mo] and [Mo]:[S]~ 1 : 2.4 for D=3 nm.
Chromatogram of clusters
Linewidth(polydispersity) comparable to chemical impurities
Oxidized to CO
Absorbance (250 nm)
t = 0
elution time (min)
Example - Destruction of an Alkyl Chloride Organic Impurity using dispersed nanosize (D = 3 nm) MoS2.
PCP UV Photooxidation Results using TiO2 (Degussa)
UV Photooxidaton using D=25 nm, SnO2 Clusters
PCP UV Photooxidation Results
Visible Light Photooxidation Results